"No rules, no circles." This is almost the same thing in the world. What are their rules for engineering? They are processes. How much do you know about the construction process of waterborne epoxy floor? First of all, we should prepare the tools needed for construction, so as to avoid panic in the construction process. In the construction process, the main tools used are: floor grinder, mixer, brush, vacuum cleaner, scraper or serrated trowel, defoaming rollers and so on. When the tools are ready, construction begins. Here, the construction of waterborne epoxy floor is completed. But 24 hours after the completion of the construction, you can wear soft soles to enter, 48 hours before normal use. And within a week can not contact water, oil, alkaline acid, silicon and other chemicals. Although the above problems are small, we must pay attention to them, otherwise they will cause unnecessary trouble for later use.第一步：环氧底涂施工
First step: epoxy primer construction
The water-borne primer curing agent and the main agent of the water-borne primer are mixed at a weight ratio of 3:1. After mixing, they are evenly stirred by an electric mixer. Then water is added at a ratio of 1:1 to mix them well and evenly. Then they are coated by rolling or spraying.
Water-borne epoxy mixed material is best used in 40 minutes. When painting, it should be thin and uniform. After coating, the surface is glossy. Where there is no gloss, it should be repaired at the appropriate time. When the water-based base coating is dry, the construction of the intermediate coating can be carried out.
Step 2: Construction of Middle-coated Mortar Layer
Firstly, water-borne curing agent and water-borne epoxy main agent were mixed at a weight ratio of 3:1, and evenly stirred by electric mixer. Then, 30% - 40% water was added to mix fully, and then a proper amount of quartz sand was added to mix.
After these are completed, the obtained materials are poured onto the ground and batched with a trowel to avoid the occurrence of knife marks. Material should be used up in 30 minutes. After the middle coated mortar layer is dried, the middle coated putty layer can be constructed.
Step 3: Construction of Middle-coated Putty Layer
The construction of this step is the same as that of medium-coated mortar layer.
Wait until the putty layer is dried and polished with a polisher to smooth the ground. After polishing, remember to clean it at least twice with a broom or vacuum cleaner
Step 4: Topcoat construction
The curing agent of waterborne epoxy topcoat and the main agent of waterborne epoxy topcoat were mixed at a weight ratio of 4:1 to stir, then 20% water was added to stir.
After mixing, the construction is carried out by scraping, and after the ground is dried, the construction is carried out by rolling or spraying.